| ||Format||Pages||Price|| |
|5||$43.00||  ADD TO CART|
|Hardcopy (shipping and handling)||5||$43.00||  ADD TO CART|
|Standard + Redline PDF Bundle||10||$51.60||  ADD TO CART|
Significance and Use
Detection and location of AE sources in weldments during fabrication may provide information related to the integrity of the weld. Such information may be used to direct repair procedures on the weld or as a guide for application of other nondestructive evaluation (NDE) methods. A major attribute of applying AE for in-process monitoring of welds is the ability of the method to provide immediate real-time information on weld integrity. This feature makes the method useful to lower weld costs by repairing defects at the most convenient point in the production process. The AE activity from discontinuities in the weldment is stimulated by the thermal stresses from the welding process. The AE activity resulting from this stimulation is detected by AE sensors in the vicinity of the weldment, which convert the acoustic waves into electronic signals. The AE instrumentation processes signals and provides means for immediate display or indication of AE activity and for permanent recordings of the data.
Items to be considered in preparation and planning for monitoring should include but not be limited to the following:
Description of the system or object to be monitored or examined,
Extent of monitoring, that is, entire weld, cover passes only, and so forth,
Limitations or restrictions on the sensor mounting procedures, if applicable,
Performance parameters to be established and maintained during the AE system verification procedure (sensitivity, location accuracy, and so forth),
Maximum time interval between AE system verification checks,
Performance criteria for purchased equipment,
Requirements for permanent records of the AE response, if applicable,
Content and format of test report, if required, and
Operator qualification and certification, if required.
1.1 This practice provides recommended guidelines for acoustic emission (AE) monitoring of weldments during and immediately following their fabrication by continuous welding processes.
1.2 The procedure described in this practice is applicable to the detection and location of AE sources in weldments and in their heat-affected zone during fabrication, particularly in those cases where the time duration of welding is such that fusion and solidification take place while welding is still in progress.
1.3 The effectiveness of acoustic emission to detect discontinuities in the weldment and the heat-affected zone is dependent on the design of the AE system, the AE system verification procedure, the weld process, and the material type. Materials that have been monitored include low-carbon steels, low-alloy steels, stainless steels, and some aluminum alloys. The system performance must be verified for each application by demonstrating that the defects of concern can be detected with the desired reliability.
1.4 Units—The values stated in either SI units or inch-pound units are to be regarded separately as standard. The values stated in each system may not be exact equivalents; therefore, each system shall be used independently of the other. Combining values from the two systems may result in non-conformance with the standard.
1.5 This standard does not purport to address all of the safety concerns, if any, associated with its use. It is the responsibility of the user of this standard to establish appropriate safety and health practices and determine the applicability of regulatory limitations prior to use.
2. Referenced Documents (purchase separately) The documents listed below are referenced within the subject standard but are not provided as part of the standard.
E543 Specification for Agencies Performing Nondestructive Testing
E569 Practice for Acoustic Emission Monitoring of Structures During Controlled Stimulation
E650 Guide for Mounting Piezoelectric Acoustic Emission Sensors
E1316 Terminology for Nondestructive Examinations
ASNT StandardsANSI/ASNT CP-189 Standard for Qualification and Certification of Nondestructive Testing Personnel
AIA StandardNAS-410 Certification and Qualification of Nondestructive Personnel (Quality Assurance Committee)
ICS Number Code 17.140.20 (Noise emitted by machines and equipment); 25.160.10 (Welding processes); 25.160.01 (Welding, brazing and soldering in general)
UNSPSC Code 73121614(Non destructive testing service)
ASTM E749 / E749M-12, Standard Practice for Acoustic Emission Monitoring During Continuous Welding, ASTM International, West Conshohocken, PA, 2012, www.astm.orgBack to Top